#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/21/4312139.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4312139
loop_
_publ_author_name
'Łukasz Dobrzycki'
'Ewa Bulska'
'Dorota Anna Pawlak'
'Zygmunt Frukacz'
'Krzysztof Woźniak'
_publ_section_title
;
 Structure of YAG Crystals Doped/Substituted with Erbium and Ytterbium
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              7656
_journal_page_last               7664
_journal_paper_doi               10.1021/ic049920z
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'Al5 Er1.4 O12 Y1.6'
_chemical_formula_weight         703.42
_chemical_name_common            'erbium-yttrium aluminium garnet (synthetic)'
_chemical_name_systematic
;
 erbium yttrium aluminium oxide (1.4/1.6/5/12)
;
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   11.9896(14)
_cell_length_b                   11.9896(14)
_cell_length_c                   11.9896(14)
_cell_measurement_reflns_used    5170
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      40.19
_cell_measurement_theta_min      4.16
_cell_volume                     1723.5(3)
_computing_cell_refinement       CrysAlisRED
_computing_data_collection       CrysAlisCCD
_computing_data_reduction        CrysAlisRED
_computing_molecular_graphics    Diamond
_computing_publication_material  SHELXTL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      295(2)
_diffrn_detector_area_resol_mean 1024
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  KM4CCD
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.1040
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       2
_diffrn_reflns_number            461
_diffrn_reflns_theta_full        40.19
_diffrn_reflns_theta_max         40.19
_diffrn_reflns_theta_min         4.16
_diffrn_standards_decay_%        2
_diffrn_standards_interval_count '50 frames'
_diffrn_standards_number         '1 frame'
_exptl_absorpt_coefficient_mu    24.788
_exptl_absorpt_correction_T_max  0.0667
_exptl_absorpt_correction_T_min  0.0270
_exptl_absorpt_correction_type   sphere
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    5.422
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       sphere
_exptl_crystal_F_000             2549
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.24
_refine_diff_density_max         1.320
_refine_diff_density_min         -0.755
_refine_diff_density_rms         0.174
_refine_ls_extinction_coef       0.00085(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.366
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_reflns         461
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.366
_refine_ls_R_factor_all          0.0486
_refine_ls_R_factor_gt           0.0160
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0292
_refine_ls_wR_factor_ref         0.0347
_reflns_number_gt                283
_reflns_number_total             461
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic049920zsi20040119_085908_09.cif
_cod_data_source_block           er50
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' tag value 'spherical' was replaced
with 'sphere' value.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_original_formula_sum        'Al5 Er1.40 O12 Y1.60'
_cod_database_code               4312139
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'z, x, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z, x'
'-y, z+1/2, -x+1/2'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z, x+1/2'
'y+3/4, x+1/4, -z+1/4'
'-y+3/4, -x+3/4, -z+3/4'
'y+1/4, -x+1/4, z+3/4'
'-y+1/4, x+3/4, z+1/4'
'x+3/4, z+1/4, -y+1/4'
'-x+1/4, z+3/4, y+1/4'
'-x+3/4, -z+3/4, -y+3/4'
'x+1/4, -z+1/4, y+3/4'
'z+3/4, y+1/4, -x+1/4'
'z+1/4, -y+1/4, x+3/4'
'-z+1/4, y+3/4, x+1/4'
'-z+3/4, -y+3/4, -x+3/4'
'x+1/2, y+1/2, z+1/2'
'-x+1, -y+1/2, z+1'
'-x+1/2, y+1, -z+1'
'x+1, -y+1, -z+1/2'
'z+1/2, x+1/2, y+1/2'
'z+1, -x+1, -y+1/2'
'-z+1, -x+1/2, y+1'
'-z+1/2, x+1, -y+1'
'y+1/2, z+1/2, x+1/2'
'-y+1/2, z+1, -x+1'
'y+1, -z+1, -x+1/2'
'-y+1, -z+1/2, x+1'
'y+5/4, x+3/4, -z+3/4'
'-y+5/4, -x+5/4, -z+5/4'
'y+3/4, -x+3/4, z+5/4'
'-y+3/4, x+5/4, z+3/4'
'x+5/4, z+3/4, -y+3/4'
'-x+3/4, z+5/4, y+3/4'
'-x+5/4, -z+5/4, -y+5/4'
'x+3/4, -z+3/4, y+5/4'
'z+5/4, y+3/4, -x+3/4'
'z+3/4, -y+3/4, x+5/4'
'-z+3/4, y+5/4, x+3/4'
'-z+5/4, -y+5/4, -x+5/4'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'x, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z'
'-z, -x, -y'
'-z-1/2, x-1/2, y'
'z-1/2, x, -y-1/2'
'z, -x-1/2, y-1/2'
'-y, -z, -x'
'y, -z-1/2, x-1/2'
'-y-1/2, z-1/2, x'
'y-1/2, z, -x-1/2'
'-y-3/4, -x-1/4, z-1/4'
'y-3/4, x-3/4, z-3/4'
'-y-1/4, x-1/4, -z-3/4'
'y-1/4, -x-3/4, -z-1/4'
'-x-3/4, -z-1/4, y-1/4'
'x-1/4, -z-3/4, -y-1/4'
'x-3/4, z-3/4, y-3/4'
'-x-1/4, z-1/4, -y-3/4'
'-z-3/4, -y-1/4, x-1/4'
'-z-1/4, y-1/4, -x-3/4'
'z-1/4, -y-3/4, -x-1/4'
'z-3/4, y-3/4, x-3/4'
'-x+1/2, -y+1/2, -z+1/2'
'x, y+1/2, -z'
'x+1/2, -y, z'
'-x, y, z+1/2'
'-z+1/2, -x+1/2, -y+1/2'
'-z, x, y+1/2'
'z, x+1/2, -y'
'z+1/2, -x, y'
'-y+1/2, -z+1/2, -x+1/2'
'y+1/2, -z, x'
'-y, z, x+1/2'
'y, z+1/2, -x'
'-y-1/4, -x+1/4, z+1/4'
'y-1/4, x-1/4, z-1/4'
'-y+1/4, x+1/4, -z-1/4'
'y+1/4, -x-1/4, -z+1/4'
'-x-1/4, -z+1/4, y+1/4'
'x+1/4, -z-1/4, -y+1/4'
'x-1/4, z-1/4, y-1/4'
'-x+1/4, z+1/4, -y-1/4'
'-z-1/4, -y+1/4, x+1/4'
'-z+1/4, y+1/4, -x-1/4'
'z+1/4, -y-1/4, -x+1/4'
'z-1/4, y-1/4, x-1/4'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Er1 Er 0.1250 0.0000 0.2500 0.00432(8) Uani 0.47 4 d SP . .
Y1 Y 0.1250 0.0000 0.2500 0.00432(8) Uani 0.53 4 d SP . .
Al1 Al 0.0000 0.0000 0.0000 0.0031(3) Uani 1 6 d S . .
Al2 Al 0.3750 0.0000 0.2500 0.0011(2) Uani 1 4 d S . .
O1 O 0.28027(18) 0.10114(17) 0.19922(19) 0.0051(4) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Er1 O1 72.17(10) 18_545 43_444 ?
O1 Er1 O1 158.64(11) 18_545 . ?
O1 Er1 O1 112.02(11) 43_444 . ?
O1 Er1 O1 112.02(11) 18_545 28_445 ?
O1 Er1 O1 158.64(11) 43_444 28_445 ?
O1 Er1 O1 72.17(10) . 28_445 ?
O1 Er1 O1 67.52(10) 18_545 16_545 ?
O1 Er1 O1 124.92(5) 43_444 16_545 ?
O1 Er1 O1 94.93(6) . 16_545 ?
O1 Er1 O1 73.98(9) 28_445 16_545 ?
O1 Er1 O1 73.98(9) 18_545 35_445 ?
O1 Er1 O1 94.93(6) 43_444 35_445 ?
O1 Er1 O1 124.92(5) . 35_445 ?
O1 Er1 O1 67.52(10) 28_445 35_445 ?
O1 Er1 O1 107.86(10) 16_545 35_445 ?
O1 Er1 O1 94.93(6) 18_545 9 ?
O1 Er1 O1 73.98(9) 43_444 9 ?
O1 Er1 O1 67.52(10) . 9 ?
O1 Er1 O1 124.92(5) 28_445 9 ?
O1 Er1 O1 73.79(10) 16_545 9 ?
O1 Er1 O1 166.50(10) 35_445 9 ?
O1 Er1 O1 124.92(5) 18_545 38_444 ?
O1 Er1 O1 67.52(10) 43_444 38_444 ?
O1 Er1 O1 73.98(9) . 38_444 ?
O1 Er1 O1 94.93(6) 28_445 38_444 ?
O1 Er1 O1 166.50(10) 16_545 38_444 ?
O1 Er1 O1 73.79(10) 35_445 38_444 ?
O1 Er1 O1 107.86(10) 9 38_444 ?
O1 Er1 Al2 143.91(5) 18_545 . ?
O1 Er1 Al2 143.91(5) 43_444 . ?
O1 Er1 Al2 36.09(5) . . ?
O1 Er1 Al2 36.09(5) 28_445 . ?
O1 Er1 Al2 83.25(5) 16_545 . ?
O1 Er1 Al2 96.75(5) 35_445 . ?
O1 Er1 Al2 96.75(5) 9 . ?
O1 Er1 Al2 83.25(5) 38_444 . ?
O1 Er1 Al2 36.09(5) 18_545 50_556 ?
O1 Er1 Al2 36.09(5) 43_444 50_556 ?
O1 Er1 Al2 143.91(5) . 50_556 ?
O1 Er1 Al2 143.91(5) 28_445 50_556 ?
O1 Er1 Al2 96.75(5) 16_545 50_556 ?
O1 Er1 Al2 83.25(5) 35_445 50_556 ?
O1 Er1 Al2 83.25(5) 9 50_556 ?
O1 Er1 Al2 96.75(5) 38_444 50_556 ?
Al2 Er1 Al2 180.0 . 50_556 ?
O1 Er1 Al1 96.28(5) 18_545 . ?
O1 Er1 Al1 33.67(5) 43_444 . ?
O1 Er1 Al1 97.18(6) . . ?
O1 Er1 Al1 126.71(6) 28_445 . ?
O1 Er1 Al1 158.55(5) 16_545 . ?
O1 Er1 Al1 79.28(5) 35_445 . ?
O1 Er1 Al1 94.64(5) 9 . ?
O1 Er1 Al1 34.35(5) 38_444 . ?
Al2 Er1 Al1 116.6 . . ?
Al2 Er1 Al1 63.4 50_556 . ?
O1 Er1 Al1 126.71(6) 18_545 38_444 ?
O1 Er1 Al1 97.18(6) 43_444 38_444 ?
O1 Er1 Al1 33.67(5) . 38_444 ?
O1 Er1 Al1 96.28(5) 28_445 38_444 ?
O1 Er1 Al1 79.28(5) 16_545 38_444 ?
O1 Er1 Al1 158.55(5) 35_445 38_444 ?
O1 Er1 Al1 34.35(5) 9 38_444 ?
O1 Er1 Al1 94.64(5) 38_444 38_444 ?
Al2 Er1 Al1 63.4 . 38_444 ?
Al2 Er1 Al1 116.6 50_556 38_444 ?
Al1 Er1 Al1 101.5 . 38_444 ?
O1 Al1 O1 86.61(10) 43_444 38_444 ?
O1 Al1 O1 93.39(10) 43_444 96 ?
O1 Al1 O1 93.39(10) 38_444 96 ?
O1 Al1 O1 86.61(10) 43_444 48_444 ?
O1 Al1 O1 86.61(10) 38_444 48_444 ?
O1 Al1 O1 180.00(18) 96 48_444 ?
O1 Al1 O1 180.00(13) 43_444 91 ?
O1 Al1 O1 93.39(10) 38_444 91 ?
O1 Al1 O1 86.61(10) 96 91 ?
O1 Al1 O1 93.39(10) 48_444 91 ?
O1 Al1 O1 93.39(10) 43_444 86 ?
O1 Al1 O1 180.00(18) 38_444 86 ?
O1 Al1 O1 86.61(10) 96 86 ?
O1 Al1 O1 93.39(10) 48_444 86 ?
O1 Al1 O1 86.61(10) 91 86 ?
O1 Al1 Er1 88.44(7) 43_444 53 ?
O1 Al1 Er1 138.31(6) 38_444 53 ?
O1 Al1 Er1 45.64(7) 96 53 ?
O1 Al1 Er1 134.36(7) 48_444 53 ?
O1 Al1 Er1 91.56(7) 91 53 ?
O1 Al1 Er1 41.69(6) 86 53 ?
O1 Al1 Er1 45.64(7) 43_444 9 ?
O1 Al1 Er1 91.56(7) 38_444 9 ?
O1 Al1 Er1 138.31(6) 96 9 ?
O1 Al1 Er1 41.69(6) 48_444 9 ?
O1 Al1 Er1 134.36(7) 91 9 ?
O1 Al1 Er1 88.44(7) 86 9 ?
Er1 Al1 Er1 113.6 53 9 ?
O1 Al1 Er1 134.36(7) 43_444 57 ?
O1 Al1 Er1 88.44(7) 38_444 57 ?
O1 Al1 Er1 41.69(6) 96 57 ?
O1 Al1 Er1 138.31(6) 48_444 57 ?
O1 Al1 Er1 45.64(7) 91 57 ?
O1 Al1 Er1 91.56(7) 86 57 ?
Er1 Al1 Er1 66.4 53 57 ?
Er1 Al1 Er1 180.0 9 57 ?
O1 Al1 Y1 138.31(6) 43_444 49 ?
O1 Al1 Y1 134.36(7) 38_444 49 ?
O1 Al1 Y1 91.56(7) 96 49 ?
O1 Al1 Y1 88.44(7) 48_444 49 ?
O1 Al1 Y1 41.69(6) 91 49 ?
O1 Al1 Y1 45.64(7) 86 49 ?
Er1 Al1 Y1 66.4 53 49 ?
Er1 Al1 Y1 113.6 9 49 ?
Er1 Al1 Y1 66.4 57 49 ?
O1 Al1 Y1 91.56(7) 43_444 5 ?
O1 Al1 Y1 41.69(6) 38_444 5 ?
O1 Al1 Y1 134.36(7) 96 5 ?
O1 Al1 Y1 45.64(7) 48_444 5 ?
O1 Al1 Y1 88.44(7) 91 5 ?
O1 Al1 Y1 138.31(6) 86 5 ?
Er1 Al1 Y1 180.0 53 5 ?
Er1 Al1 Y1 66.4 9 5 ?
Er1 Al1 Y1 113.6 57 5 ?
Y1 Al1 Y1 113.6 49 5 ?
O1 Al1 Y1 88.44(7) 43_444 53 ?
O1 Al1 Y1 138.31(6) 38_444 53 ?
O1 Al1 Y1 45.64(7) 96 53 ?
O1 Al1 Y1 134.36(7) 48_444 53 ?
O1 Al1 Y1 91.56(7) 91 53 ?
O1 Al1 Y1 41.69(6) 86 53 ?
Er1 Al1 Y1 0.0 53 53 ?
Er1 Al1 Y1 113.6 9 53 ?
Er1 Al1 Y1 66.4 57 53 ?
Y1 Al1 Y1 66.4 49 53 ?
Y1 Al1 Y1 180.0 5 53 ?
O1 Al1 Y1 45.64(7) 43_444 9 ?
O1 Al1 Y1 91.56(7) 38_444 9 ?
O1 Al1 Y1 138.31(6) 96 9 ?
O1 Al1 Y1 41.69(6) 48_444 9 ?
O1 Al1 Y1 134.36(7) 91 9 ?
O1 Al1 Y1 88.44(7) 86 9 ?
Er1 Al1 Y1 113.6 53 9 ?
Er1 Al1 Y1 0.0 9 9 ?
Er1 Al1 Y1 180.0 57 9 ?
Y1 Al1 Y1 113.6 49 9 ?
Y1 Al1 Y1 66.4 5 9 ?
Y1 Al1 Y1 113.6 53 9 ?
O1 Al1 Y1 134.36(7) 43_444 57 ?
O1 Al1 Y1 88.44(7) 38_444 57 ?
O1 Al1 Y1 41.69(6) 96 57 ?
O1 Al1 Y1 138.31(6) 48_444 57 ?
O1 Al1 Y1 45.64(7) 91 57 ?
O1 Al1 Y1 91.56(7) 86 57 ?
Er1 Al1 Y1 66.4 53 57 ?
Er1 Al1 Y1 180.0 9 57 ?
Er1 Al1 Y1 0.0 57 57 ?
Y1 Al1 Y1 66.4 49 57 ?
Y1 Al1 Y1 113.6 5 57 ?
Y1 Al1 Y1 66.4 53 57 ?
Y1 Al1 Y1 180.0 9 57 ?
O1 Al1 Er1 91.56(7) 43_444 5 ?
O1 Al1 Er1 41.69(6) 38_444 5 ?
O1 Al1 Er1 134.36(7) 96 5 ?
O1 Al1 Er1 45.64(7) 48_444 5 ?
O1 Al1 Er1 88.44(7) 91 5 ?
O1 Al1 Er1 138.31(6) 86 5 ?
Er1 Al1 Er1 180.0 53 5 ?
Er1 Al1 Er1 66.4 9 5 ?
Er1 Al1 Er1 113.6 57 5 ?
Y1 Al1 Er1 113.6 49 5 ?
Y1 Al1 Er1 0.0 5 5 ?
Y1 Al1 Er1 180.0 53 5 ?
Y1 Al1 Er1 66.4 9 5 ?
Y1 Al1 Er1 113.6 57 5 ?
O1 Al1 Er1 138.31(6) 43_444 49 ?
O1 Al1 Er1 134.36(7) 38_444 49 ?
O1 Al1 Er1 91.56(7) 96 49 ?
O1 Al1 Er1 88.44(7) 48_444 49 ?
O1 Al1 Er1 41.69(6) 91 49 ?
O1 Al1 Er1 45.64(7) 86 49 ?
Er1 Al1 Er1 66.4 53 49 ?
Er1 Al1 Er1 113.6 9 49 ?
Er1 Al1 Er1 66.4 57 49 ?
Y1 Al1 Er1 0.0 49 49 ?
Y1 Al1 Er1 113.6 5 49 ?
Y1 Al1 Er1 66.4 53 49 ?
Y1 Al1 Er1 113.6 9 49 ?
Y1 Al1 Er1 66.4 57 49 ?
Er1 Al1 Er1 113.6 5 49 ?
O1 Al1 Er1 41.69(6) 43_444 . ?
O1 Al1 Er1 45.64(7) 38_444 . ?
O1 Al1 Er1 88.44(7) 96 . ?
O1 Al1 Er1 91.56(7) 48_444 . ?
O1 Al1 Er1 138.31(6) 91 . ?
O1 Al1 Er1 134.36(7) 86 . ?
Er1 Al1 Er1 113.6 53 . ?
Er1 Al1 Er1 66.4 9 . ?
Er1 Al1 Er1 113.6 57 . ?
Y1 Al1 Er1 180.0 49 . ?
Y1 Al1 Er1 66.4 5 . ?
Y1 Al1 Er1 113.6 53 . ?
Y1 Al1 Er1 66.4 9 . ?
Y1 Al1 Er1 113.6 57 . ?
Er1 Al1 Er1 66.4 5 . ?
Er1 Al1 Er1 180.0 49 . ?
O1 Al1 O1 62.73(8) 43_444 . ?
O1 Al1 O1 31.83(7) 38_444 . ?
O1 Al1 O1 113.90(8) 96 . ?
O1 Al1 O1 66.10(8) 48_444 . ?
O1 Al1 O1 117.27(8) 91 . ?
O1 Al1 O1 148.17(7) 86 . ?
Er1 Al1 O1 145.65(3) 53 . ?
Er1 Al1 O1 59.94(3) 9 . ?
Er1 Al1 O1 120.06(3) 57 . ?
Y1 Al1 O1 147.87(3) 49 . ?
Y1 Al1 O1 34.35(3) 5 . ?
Y1 Al1 O1 145.65(3) 53 . ?
Y1 Al1 O1 59.94(3) 9 . ?
Y1 Al1 O1 120.06(3) 57 . ?
Er1 Al1 O1 34.35(3) 5 . ?
Er1 Al1 O1 147.87(3) 49 . ?
Er1 Al1 O1 32.13(3) . . ?
O1 Al1 Al1 52.37(7) 43_444 49_666 ?
O1 Al1 Al1 52.37(7) 38_444 49_666 ?
O1 Al1 Al1 127.63(7) 96 49_666 ?
O1 Al1 Al1 52.37(7) 48_444 49_666 ?
O1 Al1 Al1 127.63(7) 91 49_666 ?
O1 Al1 Al1 127.63(7) 86 49_666 ?
Er1 Al1 Al1 140.8 53 49_666 ?
Er1 Al1 Al1 39.2 9 49_666 ?
Er1 Al1 Al1 140.8 57 49_666 ?
Y1 Al1 Al1 140.8 49 49_666 ?
Y1 Al1 Al1 39.2 5 49_666 ?
Y1 Al1 Al1 140.8 53 49_666 ?
Y1 Al1 Al1 39.2 9 49_666 ?
Y1 Al1 Al1 140.8 57 49_666 ?
Er1 Al1 Al1 39.2 5 49_666 ?
Er1 Al1 Al1 140.8 49 49_666 ?
Er1 Al1 Al1 39.2 . 49_666 ?
O1 Al1 Al1 20.73(3) . 49_666 ?
O1 Al2 O1 114.33(8) 89_655 28_445 ?
O1 Al2 O1 114.33(8) 89_655 . ?
O1 Al2 O1 100.14(14) 28_445 . ?
O1 Al2 O1 100.14(14) 89_655 68_656 ?
O1 Al2 O1 114.33(8) 28_445 68_656 ?
O1 Al2 O1 114.33(8) . 68_656 ?
O1 Al2 Er1 129.93(7) 89_655 . ?
O1 Al2 Er1 50.07(7) 28_445 . ?
O1 Al2 Er1 50.07(7) . . ?
O1 Al2 Er1 129.93(7) 68_656 . ?
O1 Al2 Y1 50.07(7) 89_655 50_656 ?
O1 Al2 Y1 129.93(7) 28_445 50_656 ?
O1 Al2 Y1 129.93(7) . 50_656 ?
O1 Al2 Y1 50.07(7) 68_656 50_656 ?
Er1 Al2 Y1 180.0 . 50_656 ?
O1 Al2 Er1 50.07(7) 89_655 50_656 ?
O1 Al2 Er1 129.93(7) 28_445 50_656 ?
O1 Al2 Er1 129.93(7) . 50_656 ?
O1 Al2 Er1 50.07(7) 68_656 50_656 ?
Er1 Al2 Er1 180.0 . 50_656 ?
Y1 Al2 Er1 0.0 50_656 50_656 ?
O1 Al2 O1 144.82(6) 89_655 54_655 ?
O1 Al2 O1 57.76(11) 28_445 54_655 ?
O1 Al2 O1 100.82(7) . 54_655 ?
O1 Al2 O1 61.86(10) 68_656 54_655 ?
Er1 Al2 O1 74.38(4) . 54_655 ?
Y1 Al2 O1 105.62(4) 50_656 54_655 ?
Er1 Al2 O1 105.62(4) 50_656 54_655 ?
O1 Al2 O1 61.86(10) 89_655 77 ?
O1 Al2 O1 100.82(7) 28_445 77 ?
O1 Al2 O1 57.76(11) . 77 ?
O1 Al2 O1 144.82(6) 68_656 77 ?
Er1 Al2 O1 74.38(4) . 77 ?
Y1 Al2 O1 105.62(4) 50_656 77 ?
Er1 Al2 O1 105.62(4) 50_656 77 ?
O1 Al2 O1 148.75(8) 54_655 77 ?
O1 Al2 O1 100.82(7) 89_655 22_554 ?
O1 Al2 O1 144.82(6) 28_445 22_554 ?
O1 Al2 O1 61.86(10) . 22_554 ?
O1 Al2 O1 57.76(11) 68_656 22_554 ?
Er1 Al2 O1 105.62(4) . 22_554 ?
Y1 Al2 O1 74.38(4) 50_656 22_554 ?
Er1 Al2 O1 74.38(4) 50_656 22_554 ?
O1 Al2 O1 94.16(2) 54_655 22_554 ?
O1 Al2 O1 94.16(2) 77 22_554 ?
O1 Al2 O1 57.76(11) 89_655 45_445 ?
O1 Al2 O1 61.86(10) 28_445 45_445 ?
O1 Al2 O1 144.82(6) . 45_445 ?
O1 Al2 O1 100.82(7) 68_656 45_445 ?
Er1 Al2 O1 105.62(4) . 45_445 ?
Y1 Al2 O1 74.38(4) 50_656 45_445 ?
Er1 Al2 O1 74.38(4) 50_656 45_445 ?
O1 Al2 O1 94.16(2) 54_655 45_445 ?
O1 Al2 O1 94.16(2) 77 45_445 ?
O1 Al2 O1 148.75(8) 22_554 45_445 ?
Al2 O1 Al1 130.48(13) . 38_444 ?
Al2 O1 Er1 93.84(9) . . ?
Al1 O1 Er1 104.64(9) 38_444 . ?
Al2 O1 Y1 120.94(11) . 5 ?
Al1 O1 Y1 100.01(9) 38_444 5 ?
Er1 O1 Y1 101.58(8) . 5 ?
Al2 O1 Er1 120.94(11) . 5 ?
Al1 O1 Er1 100.01(9) 38_444 5 ?
Er1 O1 Er1 101.58(8) . 5 ?
Y1 O1 Er1 0.0 5 5 ?
Al2 O1 O1 161.63(13) . 5 ?
Al1 O1 O1 46.69(5) 38_444 5 ?
Er1 O1 O1 104.42(7) . 5 ?
Y1 O1 O1 53.90(7) 5 5 ?
Er1 O1 O1 53.90(7) 5 5 ?
Al2 O1 O1 134.61(15) . 9 ?
Al1 O1 O1 46.69(5) 38_444 9 ?
Er1 O1 O1 58.58(8) . 9 ?
Y1 O1 O1 100.84(6) 5 9 ?
Er1 O1 O1 100.84(6) 5 9 ?
O1 O1 O1 60.0 5 9 ?
Al2 O1 O1 39.93(7) . 28_445 ?
Al1 O1 O1 133.50(14) 38_444 28_445 ?
Er1 O1 O1 53.91(5) . 28_445 ?
Y1 O1 O1 123.06(13) 5 28_445 ?
Er1 O1 O1 123.06(13) 5 28_445 ?
O1 O1 O1 158.26(5) 5 28_445 ?
O1 O1 O1 103.50(12) 9 28_445 ?
Al2 O1 O1 89.86(11) . 77 ?
Al1 O1 O1 43.31(5) 38_444 77 ?
Er1 O1 O1 96.46(7) . 77 ?
Y1 O1 O1 142.57(7) 5 77 ?
Er1 O1 O1 142.57(7) 5 77 ?
O1 O1 O1 90.0 5 77 ?
O1 O1 O1 61.88(5) 9 77 ?
O1 O1 O1 94.04(12) 28_445 77 ?
Al2 O1 O1 103.30(12) . 81 ?
Al1 O1 O1 43.31(5) 38_444 81 ?
Er1 O1 O1 147.00(8) . 81 ?
Y1 O1 O1 93.53(6) 5 81 ?
Er1 O1 O1 93.53(6) 5 81 ?
O1 O1 O1 61.88(5) 5 81 ?
O1 O1 O1 90.0 9 81 ?
O1 O1 O1 136.55(10) 28_445 81 ?
O1 O1 O1 56.24(10) 77 81 ?
Al2 O1 O1 100.99(8) . 38_444 ?
Al1 O1 O1 127.37(7) 38_444 38_444 ?
Er1 O1 O1 55.08(7) . 38_444 ?
Y1 O1 O1 50.93(7) 5 38_444 ?
Er1 O1 O1 50.93(7) 5 38_444 ?
O1 O1 O1 88.17(5) 5 38_444 ?
O1 O1 O1 91.51(3) 9 38_444 ?
O1 O1 O1 77.66(7) 28_445 38_444 ?
O1 O1 O1 149.79(9) 77 38_444 ?
O1 O1 O1 144.01(10) 81 38_444 ?
Al2 O1 O1 85.85(9) . 22_554 ?
Al1 O1 O1 99.72(11) 38_444 22_554 ?
Er1 O1 O1 147.85(10) . 22_554 ?
Y1 O1 O1 53.10(5) 5 22_554 ?
Er1 O1 O1 53.10(5) 5 22_554 ?
O1 O1 O1 77.68(11) 5 22_554 ?
O1 O1 O1 137.20(12) 9 22_554 ?
O1 O1 O1 119.09(12) 28_445 22_554 ?
O1 O1 O1 115.67(8) 77 22_554 ?
O1 O1 O1 62.65(9) 81 22_554 ?
O1 O1 O1 93.36(8) 38_444 22_554 ?
Al2 O1 O1 32.84(4) . 89_655 ?
Al1 O1 O1 97.99(11) 38_444 89_655 ?
Er1 O1 O1 110.40(8) . 89_655 ?
Y1 O1 O1 137.67(11) 5 89_655 ?
Er1 O1 O1 137.67(11) 5 89_655 ?
O1 O1 O1 136.12(6) 5 89_655 ?
O1 O1 O1 119.18(12) 9 89_655 ?
O1 O1 O1 62.85(4) 28_445 89_655 ?
O1 O1 O1 60.76(11) 77 89_655 ?
O1 O1 O1 74.42(11) 81 89_655 ?
O1 O1 O1 133.80(5) 38_444 89_655 ?
O1 O1 O1 86.26(6) 22_554 89_655 ?
Al2 O1 O1 32.84(4) . 68_656 ?
Al1 O1 O1 141.08(13) 38_444 68_656 ?
Er1 O1 O1 110.40(8) . 68_656 ?
Y1 O1 O1 89.23(9) 5 68_656 ?
Er1 O1 O1 89.23(9) 5 68_656 ?
O1 O1 O1 133.67(14) 5 68_656 ?
O1 O1 O1 166.20(14) 9 68_656 ?
O1 O1 O1 62.85(4) 28_445 68_656 ?
O1 O1 O1 114.73(10) 77 68_656 ?
O1 O1 O1 98.85(11) 81 68_656 ?
O1 O1 O1 87.53(6) 38_444 68_656 ?
O1 O1 O1 56.59(11) 22_554 68_656 ?
O1 O1 O1 54.30(9) 89_655 68_656 ?
Al2 O1 Al2 87.20(8) . 81 ?
Al1 O1 Al2 74.58(7) 38_444 81 ?
Er1 O1 Al2 178.96(9) . 81 ?
Y1 O1 Al2 77.94(6) 5 81 ?
Er1 O1 Al2 77.94(6) 5 81 ?
O1 O1 Al2 74.54(8) 5 81 ?
O1 O1 Al2 120.55(6) 9 81 ?
O1 O1 Al2 127.13(4) 28_445 81 ?
O1 O1 Al2 83.44(8) 77 81 ?
O1 O1 Al2 32.38(5) 81 81 ?
O1 O1 Al2 124.81(11) 38_444 81 ?
O1 O1 Al2 32.28(5) 22_554 81 ?
O1 O1 Al2 70.46(9) 89_655 81 ?
O1 O1 Al2 70.56(8) 68_656 81 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Er1 O1 2.304(2) 18_545 ?
Er1 O1 2.304(2) 43_444 ?
Er1 O1 2.304(2) . ?
Er1 O1 2.304(2) 28_445 ?
Er1 O1 2.433(2) 16_545 ?
Er1 O1 2.433(2) 35_445 ?
Er1 O1 2.433(2) 9 ?
Er1 O1 2.433(2) 38_444 ?
Er1 Al2 2.9974(4) . ?
Er1 Al2 2.9974(4) 50_556 ?
Er1 Al1 3.3512(4) . ?
Er1 Al1 3.3512(4) 38_444 ?
Al1 O1 1.920(2) 43_444 ?
Al1 O1 1.920(2) 38_444 ?
Al1 O1 1.920(2) 96 ?
Al1 O1 1.920(2) 48_444 ?
Al1 O1 1.920(2) 91 ?
Al1 O1 1.920(2) 86 ?
Al1 Er1 3.3512(4) 53 ?
Al1 Er1 3.3512(4) 9 ?
Al1 Er1 3.3512(4) 57 ?
Al1 Y1 3.3512(4) 49 ?
Al1 Y1 3.3512(4) 5 ?
Al1 Y1 3.3512(4) 53 ?
Al1 Y1 3.3512(4) 9 ?
Al1 Y1 3.3512(4) 57 ?
Al1 Er1 3.3512(4) 5 ?
Al1 Er1 3.3512(4) 49 ?
Al1 O1 4.297(2) . ?
Al1 Al1 20.767(2) 49_666 ?
Al2 O1 1.769(2) 89_655 ?
Al2 O1 1.769(2) 28_445 ?
Al2 O1 1.769(2) . ?
Al2 O1 1.769(2) 68_656 ?
Al2 Y1 2.9974(4) 50_656 ?
Al2 Er1 2.9974(4) 50_656 ?
Al2 O1 3.304(2) 54_655 ?
Al2 O1 3.304(2) 77 ?
Al2 O1 3.304(2) 22_554 ?
Al2 O1 3.304(2) 45_445 ?
O1 Al1 1.920(2) 38_444 ?
O1 Y1 2.433(2) 5 ?
O1 Er1 2.433(2) 5 ?
O1 O1 2.634(4) 5 ?
O1 O1 2.634(4) 9 ?
O1 O1 2.714(4) 28_445 ?
O1 O1 2.795(4) 77 ?
O1 O1 2.795(4) 81 ?
O1 O1 2.852(5) 38_444 ?
O1 O1 2.921(4) 22_554 ?
O1 O1 2.974(4) 89_655 ?
O1 O1 2.974(4) 68_656 ?
O1 Al2 3.304(2) 81 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Al1 Al1 Al1 O1 3.14(8) ? . 49_666 43_444 ?
